Fabrication of one-dimensional Ag/multiwalled carbon nanotube nano-composite
© Peng and Chen; licensee Springer. 2012
Received: 13 August 2011
Accepted: 23 March 2012
Published: 23 March 2012
Composite made of multiwalled carbon nanotubes coated with silver was fabricated by an electroless deposition process. The thickness of silver layer is about 40 to 60 nm, characterized as nano-crystalline with (111) crystal orientation along the nanotube's axial direction. The characterization of silver/carbon nanotube [Ag/CNT] nanowire has shown the large current carrying capability, and the electric conductivity is similar to the pure silver nanowires that Ag/CNT would be promising as building blocks for integrated circuits.
PACS: 81.05.uj, carbon nanotubes, carbon-based materials, diamond/nanocarbon composites.
One-dimensional nanostructured metals play important roles as interconnects and nanoscale electronic devices. Silver nanowire is especially attractive due to its extremely high electric and thermal conductivities . Template-directed synthesis and the solution-phase based approach have been widely used to produce Ag nanowires [2–4]. However, pure silver nanowires are limited for metallic interconnection applications as its resistivity increase largely with the dimension decreasing due to its increased electron scattering. On the other hand, carbon nanotubes [CNTs] are known for having long mean free path (order of several microns), extremely high current densities (> 109 A/cm2 at 25°C), and high aspect ratio. The bulk composites made of metal matrix with CNTs as the reinforcement component for augmenting the metal conductivity have been extensively investigated [5–7]. However, how to fabricate and to characterize a single one-dimensional nano-composite with embedding a single CNT within the silver matrix are difficult [8, 9], and electroless silver plating process has been used to deposit silver onto multiwalled carbon nanotube [MWCNT] . In this paper, one-dimensional Ag/MWCNT nano-composite was prepared by coating the MWCNT with relatively uniform nano-crystalline silver layer using the electroless silver plating process. The electrical properties of one-dimensional Ag/MWCNT nano-composite were investigated using two terminal conductance measurements to demonstrate the resistivity and the current carrying capacity.
Results and discussion
Transmission electron microscopy observation shows that the one-dimensional Ag/MWCNT nano-composite has a relatively uniform silver coverage as shown in Figure 1a. The diameter is about 160 nm, with a deviation of about 20 nm, and the length is about 3.2 μm. The inset of Figure 1c is the selected area electron diffraction [SAED] pattern obtained from a massive bundle of one-dimensional Ag/silver nano-composites. Several continued rings and some diffraction spots that were observed in the SAED pattern indicate that the Ag/MWCNT nano-composites have a polycrystalline structure.
The distances of the lattice planes are measured using a high-resolution transmission electron microscopy [HRTEM] and shown in Figure 1d. Interplanar distance of the (111) planes which is 0.234 nm indicates that the nano-crystal silver coating possesses a face-centered cubic [FCC] structure, which are consistent with the standard lattice constant of the Ag crystal structure . Lattice fringes with spacing of 0.2046 nm which are also observed corresponds to the (200) planes in FCC crystalline silver. It can be seen that the silver coating layer is nano-crystallized without any amorphous structure .
Figure 3 (right) displays the typical linear I-V curves measured on the single, one-dimensional nanocrystalline Ag/MWCNT nano-composite wire at room temperature. More than five measurements were carried out on the sample. The resistance was calculated (based on the applied voltages and the resultant currents). The average resistance of the Ag/MWCNT is at about 75.7 Ω, and the variation among different measurements is less than 2%. Therefore, the resistivity of the one-dimensional Ag/MWCNT nano-composite is approximately 3.0 × 10-6 Ωm. It is reasonable that the resistivity of the nanocrystalline Ag/MWCNT nano-composite is higher than the bulk silver (1.5 × 10-8 Ωm) because the surface scattering of electron increases largely when the diameter is as smaller as the mean free path of the silver . Since the I-V curve is a straight line, therefore, no oxidation effects can be identified. This also agrees with the composition analysis in which no oxygen was detected. It was indicated that the resistivity of a DNA-templated silver nanowire measured by SH Park et al. was about 4 × 10-6 Ωm . It can be deduced that the one-dimensional Ag/MWCNT nano-composites have better conductivity than the DNA-coated silver nanowire. However, the resistivity of Ag/MWCNT nanowire is greater than that of a pure single crystal silver nanowire which has the resistivity of about 1.87 × 10-6 Ωm . The increased resistivity of Ag/MWCNT could be due to the multigrained structure as well as the contact resistance as well. Based on the free electron theory, the electric conductivity of metallic conductors can be described as [5, 18]: through the free electron gas theory , where n is the electron density of state, is the mean free path, me is the mass of electron and VF is the Fermi velocity. The electrical conductivity is proportional to the mean free path, i.e., the longer the mean free path, the higher the conductivity will be. The silver coating on the sidewalls of MWCNTs forms composite couplings to electronic states through the charge transfer interaction from the silver ions to MWCNTs . The metallic MWCNTs can be ballistic conductors and have a mean free path of 0.5 μm equaling with the length of the tube . The embedding MWCNT in a silver matrix facilitates electron transfer along with the ballistic transport from end to end, thereby prolonging the electron's mean free path of nano-composite ten times of the silver . The low resistivity of one-dimensional Ag/MWCNT nano-composite silver nanowire can attribute to the longer mean free path of MWCNT. The current density t was calculated to be about 6.56 × 107 A/cm2 at the voltage of 100 mV through the t = I/S, where S is the cross sectional area and I is the current. The current can be kept stable during the 20 min measurement under the constant voltage of 100 mV. Since electromigration occurring in Ag interconnects at the current density of 106 to 107A/cm2 , and the metallic MWCNT can stand electric current density (along axis) more than 1,000 times greater than that of silver; therefore, it is clear that integration of MWCNTs in nano-composites would be good to counter electromigration.
As a summary, MWCNTs coated with about 40 to 60 nm of relatively uniform and continuous nano-crystalline silver layer were fabricated using an electroless silver plating process. The two-terminal I-V electrical measurements conducted have demonstrated that the one-dimensional nano-crystalline Ag/MWCNT nano-composite has low resistivity and high current carrying capacity at room temperature. The electrical conductivity of MWCNTs has been enhanced by depositing pure crystal silver on their surface, and the maximum current carrying capacity of silver have been enhanced by embedding with MWCNT. Therefore, the one-dimensional nano-crystalline Ag/MWCNT nano-composite wires are promising to be used as interconnects in the area of nanoelectronic device.
This work was supported by the Natural Science Foundation of USA and Natural Science Foundation of China (grant no. 51002030). YP also acknowledges the financial support from Southeast University for excellent young faculty.
- Hong BH, Bae SC, Lee CW: Ultrathin single-crystalline silver nanowire arrays formed in an ambient solution phase. Science 2001, 294: 348. 10.1126/science.1062126View ArticleGoogle Scholar
- Yang R, Sui CH, Gong J, Qu LY: Single-crystal silver nanowires: preparation and surface-enhanced Raman scattering (SERS) property. Mater Lett 2007, 61: 900. 10.1016/j.matlet.2006.06.009View ArticleGoogle Scholar
- Barbic M, Mock JJ, Smith DR, Schultz S: Single crystal silver nanowires prepared by the metal amplification method. J Appl Phys 2002, 91: 9341. 10.1063/1.1476071View ArticleGoogle Scholar
- Choi JS, Sauer GD, Nielsch K, Wehrspohn RB, Gsele U: Hexagonally arranged monodisperse silver nanowires with adjustable diameter and high aspect ratio. Chem Mater 2003, 15: 776. 10.1021/cm0208758View ArticleGoogle Scholar
- Hjortstam O, Oderholm SS, Dai H: Can we achieve ultra-low resistivity in carbon nanotube-based metal composites? Appl Phys A 2004, 78: 1175. 10.1007/s00339-003-2424-xView ArticleGoogle Scholar
- Feng Y, Yuan HL, Zhang M: Fabrication and properties of silver-matrix composites reinforced by carbon nanotubes. Mater Charariz 2005, 55: 211. 10.1016/j.matchar.2005.05.003View ArticleGoogle Scholar
- Chen XH, Xia JT, Peng JC, Li WZ, Xie SS: Carbon-nanotube metal-matrix composites prepared by electroless plating. Comp Sci & Tech 2000, 60: 301.View ArticleGoogle Scholar
- Peng YT, Chen QF: The synthesis of a copper/multi-walled carbon nanotube hybrid nanowire in a microfluidic reactor. Nanotechnology 2009, 20: 235606. 10.1088/0957-4484/20/23/235606View ArticleGoogle Scholar
- Jankovic LB, Gournis DM, Trikalitis PN: Carbon nanotubes encapsulating superconducting single-crystalline tin nanowires. Nano Lett 2006, 6: 1131. 10.1021/nl0602387View ArticleGoogle Scholar
- Qiu LH, Pol VG, Wei Y, Gedanken AH: Sonochemical decoration of multi-walled carbon nanotubes with nanocrystalline tin. New J Chem 2004, 28: 1056. 10.1039/b314397jView ArticleGoogle Scholar
- Feng Y, Yuan HL: Electroless plating of carbon nanotubes with silver. J Mater Sci 2004, 39: 3241.View ArticleGoogle Scholar
- Peng YT, Hu YZ, Wang H: Tribological behaviors of surfactant-functionalized carbon nanotubes as lubricant additive in water. Tribo Lett 2007, 25: 247. 10.1007/s11249-006-9176-7View ArticleGoogle Scholar
- American Electroplaters and Surface Finishers Society: The fundamental aspects of electroless nickel plating. In Electroless Plating Fundamentals and Applications. Edited by: Mallory GO, Hajdu JB. New York: Noyes Publications/William Andrew Publishing; 1990.Google Scholar
- Bhattacharyya S, Saha SK: Silver nanowires grown in the pores of a silica gel. Appl Phys Lett 2000, 77: 3770. 10.1063/1.1327278View ArticleGoogle Scholar
- Huang Q, Lilley CM, Bode M: An in situ investigation of electromigration in Cu nanowires. Appl Phys Lett 2009, 95: 103112. 10.1063/1.3216836View ArticleGoogle Scholar
- Liu SW, Wehmschulte RJ, Lian GD, Burb CM: Room temperature synthesis of silver nanowires from tabular silver bromide crystals in the presence of gelatin. J Sol Sta Chem 2006, 179: 696. 10.1016/j.jssc.2005.11.021View ArticleGoogle Scholar
- Park SH, Prior MW, Thomas H, LaBean : Optimized fabrication and electrical analysis of silver nanowires templated on DNA molecules. Appl Phys Lett 2006, 89: 033901. 10.1063/1.2234282View ArticleGoogle Scholar
- Kittel C: Introduction to Solid State Physics. Sixth edition. New York: Wiley; 1986.Google Scholar
- Fujimori MS, Heike SJ, Hashizume TH: Electrical conduction of Ag nanowire fabricated on hydrogen-terminated Si(100) surface. J J Appl Phys 2006, 45: 2184.View ArticleGoogle Scholar
- Andriotis AN, Menon M, Froudakis GE: Various bonding configurations of transition-metal atoms on carbon nanotubes: their effect on contact resistance. Appl Phys Lett 2000, 76: 3890–3892. 10.1063/1.126811View ArticleGoogle Scholar
- Yoshimoto S, Murata Y, Hobara R, Matsuda I, Kishida M, Konishi H, Ikuno T, Maeda D, Yasuda T, Honda S, Okado H, Oura K, Katayama M, Hasegawa S: Electrical characterization of metal-coated carbon nanotube tips. J J Appl Phys 2005, 44: L1563.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.